Sep 15, 1994 - Karl Amundson,* Eugene Helfand, Xina Quan, and Steven D. Hudson. AT&T Bell Laboratories, Murray Hill, New Jersey 07974. Steven D. Smith.
Macromolecules 1994,27, 6559-6570
Alignment of Lamellar Block Copolymer Microstructure in an Electric Field. 2, Mechanisms of Alignment Karl Amundson,* Eugene Helfand, Xina Quan, and Steven D. Hudson AT&T Bell Laboratories, Murray Hill, New Jersey 07974 Steven D. Smith The Procter and Gamble Company, Cincinnati, Ohio 45239 Received May 5, 1994; Revised Manuscript Received August 12,1994’ ABSTRACT Alignment of lamellar block copolymer microstructurein an electric field was studied. Two mechanismsof alignment are considered selective electric-field-induceddisordering and alignment through movement of defects. The latter mechanism is supported by the findings that, in an aligned sample,defect structures exhibited a highly anisotropic arrangement and were spatially clumped. An analysis of fieldinduced forces on disclination lines and defect walls is presented. Also, defect interactions are considered. Through the interplay between these forces, the alignment process, the kinetics of alignment,and clumping of defects can be rationalized.
1. Introduction Alignment of block copolymer microstructure by deformation or flow has been studied extensively.14 Recently, we have reported on the alignment of lamellar block copolymer microstructure in the relatively weak aligning force induced by an electric field.gJO The most recent paperlo focused primarily upon alignment kinetics. Here, we report on the morphology of the microstructure in aligned block copolymers and what it indicates about the mechanisms of alignment. The driving force for alignment is the anisotropic free energy of a block copolymer with a lamellar microstructure. In an electric field, the electrostatic contribution to the free energy density of a block copolymer with lamellar morphology can be expressed to lowest order aslo
3 is the free energy, 30is the free energy in the absence of an electric field, and Y is the volume. CDis the dielectric constant in the limit of vanishing stationary composition pattern, 0 is the sensitivity of the dielectric constant to composition, = dc/d#, and ( e ) is a space-averag? dielectric constant (defined more precisely in ref 10). #(r) is the compositional order parameter associated with the stationary composition pattern, and &, is the unit wave vector of the lamellae. 6, is the unit vector in the direction of the applied field, Eo. This expression results from a perturbation expansion in the composition patternlo and is strictly valid only when the quantity
nism are drawn from microscopicexamination of the defect structures in an aligned block copolymer sample.
11. Experimental Section Polystyrene-poly(methy1 methacrylate) diblock copolymer (PS-PMMA) sampleswere synthesized anionically. The polymer in this study has a molecular weight average of 37 000 (polydispersityindex 1.08)and is 53 vol % polystyrene, as determined by lH NMR with consideration to density. The order-disorder transition (ODT)was determined rheologically and optically to be in the range 251-256 O C . l l The sample cell was described in a previous paper.1° It is heated by flowing hot nitrogen and allows for simultaneous application of an electric field and birefringence measurement, although birefringence measurements were not used in the study discussed in this paper. The PS-PMMA block copolymer sample was heated to 247 “C (several degrees below the order-disorder transition),at which point an 18 kV/cm electric field was applied. The sample was held at that temperature for approximately 10 min, then cooled 3-4 “C/min to room temperature. The field was applied until the sample cooled to below the glass transition. The small angle X-ray scattering pattern of the sample after alignment is shown in Figure 1. The X-ray beam direction was orthogonal to the direction the electric field was previously applied. The SAXSpattern reveals strongalignment of lamellae in the lowest-energy orientation,where their normal vectors are orthogonal to the electric-field direction. Microtome slices were taken from the aligned sample (far from any surfaces),stained with ruthenium tetraoxide, and viewed with a transmission electron microscope. The two orientations of slice planes with respect to the direction of electric-field application are shown in Figure 2. Some slice planes were perpendicular to the electric field and are referred to as “perpendicularslices”. Other slice planes contained the electric field direction and are referred to as “parallel slices”.
111. Morphology of the Aligned Sample is small. The first term on the right of eq 1 is anisotropic. The microstructural orientation with lowest free energy is such that the Fourier components of the composition pattern have wave vectors (in the direction 6,) orthogonal to the applied field. In this paper, the mechanisms by which anisotropic free energy gives rise to aligned microstructure are explored. Clues about the alignment mecha-
* Abstract published in Advance ACS Abstracts, September 15, 1994. 0024-929719412227-6559$04.50/0
Figure 3 shows portions of typical transmission electron micrographs of “parallel” and “perpendicular”slices. The two types are quite distinct. For perpendicular slices, the dark and light stripes are usually of fairly uniform period. Also, the periodicity of the stripes is usually in approximate agreement with the 23 nm periodicity of the lamellae, as determined by SAXS. This is consistent with the nearly orthogonal intersection of the slice plane with the lamellae, as expected for a field-aligned sample. The orientation of 0 1994 American Chemical Society
6560 Amundson et al.
Figure I . Small angle X-ray scattering pattern from the block copolymer sample after alignment in the electric field. The X-ray beam was orthogonal to the applied field direction which is indicated by the arrnw. The two peaks arise from scattering off
the lamellar microstructure. Thin arcsnear the beamstop result from beam leakage and imperfect heam alignment. "perpendicular slice": slice plane IEo
\"parallel slice": slice plane contains Figure2 Orientation ofsliceplaneswith respect tothedirection of the applied field.
the lamellae meanders in the slice plane, however. This is also expected, since all lamellar orientations for which the normal vector is in the plane perpendicular to the electric field make up a degenerate set of lowest-energy orientations. In addition, four classes of defect structures are identifiable. disclination lines and defect walls are most prevalent. -1/2 disclination lines and isolated edge dislocations are also observed, but are rarer. These defect structures in smectic-A systems are discussed in books by de Gennes and Prost12 and K l e ~ n a n 'and ~ in numerous reports."" Disclination lines are lines of singularity in the &q field. They are characterized by a * T rotation of the lamellar wave vector upon counterclockwise travel along a loop that circumscribes a type * I / Z disclination fine. The points of intersection of some disclination lines with theslice planeareindicated inFigure3a. Walldefects are planes across which the microstructural pattern makes adiscontinuous jump in orientation. Linesof intersection
Macromolecules, Vol. 27,No.22, 1994 between wall defects and the slice plane are also indicated in Figure 3a. Representative micrographs of 'parallel" sections are shown in Figures 3b,c. Typical views are of fairly uniform patterns, as in Figure 3b and the lower right and upper left of Figure 3c. Striations are primarily along the direction of the applied field, asexpected for a field-aligned sample. The repeat distance of the light and dark bands are commonly larger than the 23 nm periodicity of the lamellae, indicative of nonorthogonal intersection of the slice with lamellae. In distinction to Figure 3a, sharp intersections with disclination lines are not prevalent; instead it amears that the traiectories of disclination lines in the aligneh sample are prehominantly in the direction of the electric field. Also, 'disturbances" such as that running through the center of Figure 3c are common. Typically, these regions are long in the direction of the electric field and have a width on the order of 1pm. In gross view, they are regions of a very coarse pattern, indicating a very shallow intersection of the slice plane with the lamellae. It is likely that these features arise from a disclination line with a trajectory approximately in the slice plane, but offset from the slice plane, as is illustrated in Figure 2. The coarse pattern is similar to a wood grain pattern. A more detailed analysis of these features reveals additional complexity; there is a high density of shortrange defects in these regions. The strong curvature and sharpjumps in lamellar orientation indicate a high density of line and wall defects. The formation of these regions is likely due to defect interactions and defect pinning, as will be discussed in the next section. As just stated, in the aligned material, disclination lines rune predominantly in the direction of the applied field. In addition, defect walls are anisotropically arranged in the aligned sample. This is best understood by first defining a rotation axis for a wall defect. A rotation plus a translation is required to map the lamellar pattern on one side of a wall defect to the other. We refer to the axis of rotation as the rotation axis for the wall. If the wall contains its rotation axis, it is a bend wall, and if the axis is perpendicular to the wall, it is of twist character. If the rotation axis is somewherein between, the wall is of mixed character. In the field-aligned sample, the rotation axes of the wall defects are predominantly aligned along the direction of the applied field,&.. Thus, walls with normals parallel to C. have primarily twist character, while walls with normals nearly perpendicular to 6. have primarily bend character. Examples of bend walls are indicated in Figure 3a.
IV. Mechanisms of Alignment In this section, two possible alignment mechanisms are examined. First, the destabilizing effect of the electric field on the microstructure in disfavored orientations will be considered. Next alignment by movement of defect structures will be considered. A. Alignment by SelectiveDisordering. Anelectric field has an anisotropic destabilizing effect on lamellar microstructure (see eq 1.1). It is then conceivable that microstructural alignment is achieved by selective disordering in regions where the lamellae are in "disfavored" orientation. This postulate is quantitatively treated here using the thermodynamic potential of Fredrickson and Helfand.l* The conclusion is that the effect is far too weak to be operative. However, in stronger but experimentally attainable fields, thismechanism isquite possible. This analysis will consider only weak segregation, and the ordered phase composition pattern will be described
Macromolecules, Vol. 27,No. 22, 1994
Figure3. Transmissionelectron micrograph? 111 mi